Fig. 3.1 Schematic representation of intra- and inter-modal dispersion for a pulse of light propagating in two modes.

2. The Dispersion Relations

The scalar propagation constant is given by eqn. (2.39).

Because we are using the weakly-guiding approximation, so that A << 1 , we may write

kn (1 - A — )

**p n v ** **'**

**G O ** **y** 2 (3.1)

We define the dimensionless group delay as dß r _ dn U dU r,_ dA

as r . an u au **r .**

— = (n + k — — **Tr **— Ikn —

*r\ir* L dk V dV ^ *Alr*

(3.2)

where we have set n = nCQ for simplicity. The conversion of eqn. (3.2) to practical units is given in the Appendix.

As we shall see later, we can neglect terms of order

A(k/n)(dn/dk) and (dA/dk) and write the group delay for each mode as

**t** = N + nAT _{(3.3)}
where
N = N (A ) = n + k ~~ = n(\)
ak
dn( A )
dA

is the group index and

T e T(V) **U2**
*\J2*
U dU
V dV
(3.4)
(3.5)

is the normalized modal group delay [1]. (The equation for T in reference [1] should be corrected by a term A [2], which gives eqn. (3.5).)

The intra-modal dispersion, or total dispersion, of a mode is the spread in the group delay due to the small spread in wavelength of the source of transmission, and here we define it as

St = (t/x) sx (3.6a) t

**t****c**** 421**

dk2
D( X ) dT
+ nAV dV ### (3.6b)

where D(X) = 2k### 4a

* — = X2 — (3.7) dk2 dX2is the material dispersion of the bulk material from which the fiber is made, and V(dT/dV) is the waveguide dispersion, and depends only on the geometry of the guide. The total dispersion can then be expressed as a combination of material and waveguide dispersions:

t = t +

m nA tw (3.8)

in reference [31 the complete expression for t is derived (i.e., the derivative with respect to k of eqn. (3.2)) where it is shown that profile dispersion, i.e., terms with coefficient dA/dk , are small and can be neglected. In the Appendix we compare eqn.(3.8) to the numerical derivative kd28/dk2, with 3 given by eqn. (2.39), over a range of wavelengths. The results are given in figure 3.12. We find eqn. (3.6) to be an excellent approximation to the intra-modal dispersion of a fiber.

3. Material Dispersion

In this section we will investigate the variation of the refractive index, profile height, and material dispersion with respect to wavelength. Throughout this thesis we consider an optical fiber in which the refractive index of the cladding, n , is composed of pure silica, and the refractive index of the core, nQ 0 , is composed of GeO, doped silica. We find that there is a linear relation between nCQ and the amount (molar percent, m) of GeO, for any given wavelength. Throughout this work we will be mainly concerned with the wavelength range

0.5 um < X < 1.5 urn .

The experimental variation of refractive index with wavelength can be fitted to a three term Selimeir dispersion relation of the form

where are constants related to material oscillator strengths and * i.* are
the oscillator wavelengths. The dispersion can then be found by direct
differentiation:
(3.9)

**n is 1 3? \3**(3.10a)

**i**

**d X 2**

**n**

**i = 1 33 \ 6**

**i =i= 1 3? X 1***

**n is 1 3? X 3**

**l**

**i**

**i**(3.10b)

We use the experimental results of reference [4], in which the values of A^ and 2, are determined for 5 different amounts of Ge02 , including the pure silica case. We define the quantity m to be the molar percent of G e 0 2 dopant in the core, and consider m = 0%, 3.1*, 5.8$ and

*1*

**.***9*

*Similar data is available for other dopants [5].*

**%.**In figure 3.2 we use eqns.(3.9) and (3.10) and plot a) n(x), b) X dn/dX and c) X 2 dn/dX2 against wavelength for the different m. In fig. 3.2(d) we plot n, against X over a large range of wavelengths and find that the Sellmeir equation (3.9) breaks down for X < 0.3 and X 1 8.0 . We note that material dispersion (eqn.(3.7)) is zero at around X = 1.3 um .

As mentioned previously, we consider fibers in which the cladding is considered to be pure silica (0 GeO, ). Thus the profile height is directly related to the amount of dopant in the core. In fig. 3.3 we plot a) A and b) x dA/dX against wavelength for different amounts of G e 0 2 in the core. We note that fig. 3.2(b) and fig. 3.3(b) justify our approximation of eqn. (3-3) where terms of order

A(k/n)(dn/dk) and k(dA/dk) are neglected.

In fig. 3.4 we plot a) n and b) D(x) = X 2 d 2n/dx2 against the amount of GeO, for several values of wavelength. The experimental points are from ref. [4] For a wide range of wavelengths there is a linear relation between n, D(x) and the molar percent of Ge02 dopant in the core. Thus we can write a simple linear relation to find the value of n, D and A at any wavelength X and any molar percent m of Ge02 :

**--- m-O.0%**
**--- m=3.5%**
**--- m«S.8%**
**--- m=*7.9%**
**c 1.46**

**A.(jum) **

**A. (jam)**

**0.05-**

**Fig. ** **3.2** Material dispersion data against wavelength for different
concentrations of GeO, dopant.

**zx**

**zx**

**n**

**n**

** x**

**v**

(a)
1.0
**0.0**

**f**

**---**

**L __ _**

**2.0**

**n**

**\****Ö**

**t**

**$ 1-0'****m=3.5%----**

**nd :**

**:**

**m*5.8%----**

_{0.0}**m=7.9%---**

**0.50**

**0.75**

**Fig. 3.3**1.00

**A. (urn)**\

**\**

**\**

**\**

**\**

**\**

**\**

**\**-

**1.25**

**1.50**

**0.50**

**0.75**1.00

**X(jim )**

**1.25**

**1.50**

Profile height against wavelength. The cladding is assumed pure
silica (m = *0 % )* and the core has different concentrations of

Ge02 dopant.

n(X,m) = n(x,0) + {n(X,7.9) - n(X,0)} m/7.9 (3.11a)

D (X ,m ) = D(X,0) + {DC X ,7.9) - D(X,0)} m/7.9 (3.11b)

and hence

**A ( X , m ) ** = *~* {1 - n- (-U ° I } . (3.11c)
n 2(*X*,m)

Equations (3*11) are the basis for evaluating the theoretical

results on four-photon mixing and mode propagation that will be presented

later. In the Appendix we express our dimensionless dispersion D(X) in

practical units.

**4. ** **Waveguide Dispersion**

We are interested in the waveguide part of the intra-modal

dispersion relation (3.8):

? tJ dUx

V d V J (3.12)

For the singly clad step-profile fiber one can differentiate the

**Z****. **2**.**1**»***

eigenvalue equation (-g —**19**) with respect to V to obtain
K2(W)

**:**

**Vi(H) K**1**+i(w)}**

(3.13)
t
w 2** —** { ( 1** -**2**< ) < + —** (1** - —** (1** - <)) ** x
V2 W 2 V2
WK (W) WK (W)

### ^Ka+1(w) +

k### “ 7T

w### )^1<

### ^ + 2<^'

where (3.14) K*(W)### K = :V l (W)

**K**1

**+ ,(W) •**

For the fundamental mode (i=0) eqn. (3-14) reduces to the result of

reference [6]. Usually, only the waveguide dispersion of the fundamental mode is important, because in few-mode fibers the inter-modal and material

**r**

disp^sion will dominate.

For the clad power-law profile and W-fiber the waveguide

dispersion t is evaluated numerically, with eigenvalue U specified in

Section 2-3. In fig. 3.5(a) the fundamental mode waveguide dispersion t is plotted against V for the clad power-law profile with several values of profile parameter q. ( q = « is the step-profile, given by eqn. (3.14)), and in fig. 3.5(b) we plot t against q for a fixed value of V = 2.2.

In figure 3.6 we consider the fundamental mode t for the W-
fiber. Fig. 3.6(a) is a plot of t against V for several values of radius
ratio Q and fixed profile ratio P = 0.5 (refer to Section 2-3(c) for
definitions of P and Q ) . Fig. 3.6(b) shows t againso Q for several
values of P and fixed V = 2.2. As mentioned earlier, variation of V is
really a variation in wavelength, so one may expect the profile ratio P to
change with a change in * X* . However, as fig. 3.4(b) shows, the variation
in the difference between any two A's is negligibly small, so the ratio P
is effectively a constant.

In Section 3-6 we examine the intra-modal dispersion in the wavelength region where tm is very small, so that t plays a major role in determing the zero-dispersion wavelength.

### 2

---### 0

### 1

### 2

### 3

### V=2.2

### q

Fig. 3.5 Waveguide dispersion of the fundamental mode for the clad power law profile. (a) t vs. V for different q (q = ® is the step profile); and (b) t vs. q for a fixed V = 2.2.

**P=0.5**

### 2 .0

----**0 **

**1**

**2**

**3**

**V=2.2**

**0.50 H**

**P=0.25**

**— P=0.50**

**0.00J**

**Q**

Fig. 3.6 Waveguide dispersion of the fundamental mode for the W-fiber. (a) t vs. V for a fixed P and different radius ratio Q; and

**w**

(b) tfI vs. Q for a fixed V = 2.2 and several values of P.

5. Modal Group delay

We now consider the few mode case dispersion is the major cause of pulse spreading, is the difference in group delays of the modes, fiber the modal group delay is

in which inter-modal Inter-modal dispersion For the step-profile

T
im
**U2**
**V**2
*{-*

**Kjj(W)**

**Vl(W)**

K 1+1(W>
- 1) (3.15)
where we have substituted eqn. (3.13) into eqn. (3.5). For the clad power-law profile and W-fiber eqn. (3.5) is evaluated numerically.

In figure 3.7 we plot T for the first five modes against normalized frequency V. Figure 3.8(a) is a plot of T against V for the clad-power law profile for several values of q, and fig. 3.8(b) is a plot of T against q for several values of V.

In figure 3.9 we consider the W-fiber, and in (a) we plot T against V for a fixed Q and several values of P, while in (b) we plot T against Q for fixed P and several values of V.

In Chapter 5 we shall see that the difference in modal group delay is the key to phase matching the stimulated four-photon mixing process on few mode optical fibers, and understanding experimental results.

**0**

**2**

**4**

**6**

**8**

**V**

### (b)

**— V=6**

### q

Fig. 3.8 Modal group delay for the clad power-law profile. (a) T vs. V

### Q=1.5

### P=0.25

### - - P=0.50

### P=0.5

### --- V=6

**Q**

Fig. 3.9 Modal group delay for the W-fiber. (a) T vs. V for different P and fixed Q; and (b) T vs. Q for different V and fixed P.

6. The Zero-Dispersion Wavelength

In Chapter 5 we will see that phase-matching the stimulated four-photon mixing process on single mode fibers depends critically on the zero-dispersion wavelength. In this Section we review the concepts and basic design considerations for achieving zero-dispersion operation on optical fibers.

In Sections 3-3 and 3-4 we looked at material and waveguide dispersion seperately. In this section we examine the total intra-modal dispersion (i.e. eqn. (3.6)) for a single mode fiber in the region where material dispersion t is small and the dominant effect is the waveguide dispersion. We consider some specific examples.

In figure 3.10 we give a typical loss curve for a Germanium
doped core optical fiber. The peak at X = 1.4 urn is due to •**water **OH
ions. Thus a fundamental design principle is to operate at longer
wavelengths to reduce losses, but avoid the OH peaks. 1.3 um and 1.55 um
are ideal operating wavelengths.